Experiments-Structure and Mechanical Properties of the Turtle Shell
The multiscale structure, materials properties, and mechanical responses of the turtle shell (Terrapene carolina) were studied to understand the fundamental knowledge of naturally occurring biological penetrator-armor systems. The structure observation and chemical analysis results revealed that the turtle shell carapace comprises a multiphase sandwich composite structure of functionally graded material having exterior bone layers and a foam-like bony network of closed-cells between the two exterior bone layers. Although the morphology was quite different, the exterior bone layers and interior bony network possessed comparable hardness and elastic modulus values of ~1 GPa and ~20 GPa, respectively. Compression and flexure test results showed a typical nonlinear deformation behavior recognizant of man-made foams. The mechanical test results revealed that the interior closed-cell foam layer plays a significant role on the overall deformation behavior of the turtle shell. The finite element analysis simulation results showed comparable agreement with the actual experimental test data. This systematic study could provide fundamental understanding for structure-property phenomena and biological pathways to design bio-inspired synthetic composite materials
Corresponding Author: Hongjoo Rhee
Structure observations on the turtle shell revealed a multiphase composite material that is arranged by a multiscale hierarchy. Such a multiscale hierarchical structure of the turtle shell carapace is depicted in Fig. 1. The turtle shell comprises a series of connected individual plates covered with a layer of horny keratinized scutes (Fig. 1a–b). The scutes are made up of a fibrous protein called keratin that also comprises the scales of other reptiles . These scutes overlap the seams between the shell bones and serve to reinforce the overall protection to the shell. The carapace is made of a sandwich composite structure of functionally graded material (FGM) having relatively denser exterior layers and an interior fibrous foam-like layer (Fig. 1c–d). SEM micrographs clearly revealed such fibrous structure inside of the cell (Fig. 1e–f).
The internal structure of the turtle shell was nondestructively observed by using an X-ray computed tomography (CT) and obtained images are provided in Fig. 2. The X-ray CT was carried out by using a v|tome|x by phoenix|x-ray. The X-ray CT images clearly showed that the pores within the interior foam-like layer of the turtle shell carapace were closed-cell type and randomly distributed. In addition, the results obtained from the in-house image analyzer software revealed that the porosity levels of the relatively denser exterior, interior foamlike layer, and whole turtle shell carapace including all three layers were 6.86%, 65.5%, and 48.9%, respectively.
Figs. 3 and 4 show the microstructure observation and chemical analysis results obtained from various surfaces of the turtle shell. Three different layers of the outermost keratin layer, right underneath the keratin layer, and the inside surface of the turtle shell carapace were observed and analyzed by using an SEM and an energy dispersive X-ray (EDX) spectroscopy technique, respectively. These layers have different surface microstructures and chemical compositions. The EDX analysis showed that the outermost keratin layer mainly consists of carbon (C), oxygen (O), nitrogen (N), and sulfur (S) that are main constituents of the protein. The result is not surprising since the keratins are a family of fibrous structural proteins, also called scleroproteins. Unlike the outermost keratin layer, right underneath the keratin layer and the inside surface of the turtle shell carapace contained abundant additional minerals as indicated by the presence of calcium (Ca, 15–20 wt.%), phosphorous (P, 7–10 wt.%), sodium (Na), chlorine (Cl), and magnesium (Mg) that are known to be main components of the bone.
The microstructures and chemical analysis results obtained from different locations of the fracture surfaces of the turtle shell carapace are provided in Figs. 5 and 6. The chemical compositions obtained from the exterior layers and the network (e.g. closed-cell wall) region within the foam-like interior layer were quite similar to those can be found in Fig. 4b–c. The fibers inside of the closedcell also showed an accordant chemical composition (Fig. 6b), which implies that they include “bony” fibers. The microstructure observation and chemical analysis results obtained from various locations of the turtle shell clearly revealed that the turtle shell carapace is made of a sandwich composite structure having exterior lamellar bone layers and an interior bony network of closedcell fibrous foam layer.
Experimental results obtained from the nano- and microindentation tests on the side surfaces of the turtle shell carapace are provided in Fig. 7. The results showed that the exterior layers and interior bony closed-cell walls possess comparable hardness and modulus values. Hardness and elastic modulus values obtained from the nano-indentation tests ranged from 0.8–1.1 GPa and 18.3– 24.8 GPa, respectively; whereas, the average hardness value obtained from the Vickers hardness tests was about Hv100 that corresponds to 0.98 GPa. There were small variations in hardness and elastic modulus values from experiments due to the roughness of the specimen. The nano-indentation test results reflect highly localized micromechanical properties that may contain porous or impurities in its texture. Since the regions of indentation are so small that local impurities or defects can induce uncertainties in the measurements. This effect is minimized under Vickers hardness test set-up and the exterior layers and closed-cell walls within an interior layer possessed comparable hardness values.
For quasi-static compression tests, two different types of coupon specimens including all three layers and then only a bony exterior layer were prepared. The effect of strain rate on the mechanical behavior of the turtle shell was compared with respect to the different density levels and the raw data obtained from the tests is illustrated in Fig. 8a. The lower five curves (represented by lines with symbols) were obtained from the test specimens including all three layers (two exterior and an interior layers); whereas the upper six curves were obtained from the specimens only containing a relatively denser exterior layer. Top three curves (in symbols) among those six curves were obtained from thinner specimens and the bottom three curves (in lines) represent thicker specimens. The thickness difference between those two regimes was about 15%. The favorable deformation mechanism of the turtle shell carapace under quasi-static compression test conditions can be explained by importing that of synthetic foams and/or honeycombs since fundamental structures of the test specimens are similar to those of such cellular solids. At small strains, the specimens were deformed in a linear elastic manner due to the cell wall bending. Soon after the initial linear elastic deformation, a plateau of deformation was reached, because of the buckling of the cell walls. After such a plateau of deformation, another period of linear deformation was proceeded since a densification occurred resulting in a rapid increase of compressive stress. When comparing the specimens containing the exterior region only, the thicker specimens showed a similar deformation yet much weaker behavior than those can be observed in the specimens including all three layers; whereas the thinner specimens showed almost a linear compressive deformation behavior simply because of the density and structure differences. Most of discernible pores within exterior layer are distributed near the region between the exterior layer and interior foam-like layer. Fig. 8b provides the comparison of specific energy absorption obtained from the quasi-static compression test results (Fig. 8a). Density and porosity levels of the test specimens were already considered in this normalized data. The energy absorption ability of the turtle shell carapace increased with increasing strain rate for a given density level. The composite layers including all three layers showed better energy absorption ability compared to the exterior layer for any given strain rate. In addition, such composite layers possessed a considerable amount of plateau of deformation that is a model index of good energy absorbing materials. The combining information of these two plots in Fig. 8 is very important to design the optimum energy absorbing composite material. For example, composite foam materials can be tailored to give the best combination of properties for a given package by choosing the right combination of the cell wall materials, relative density, reinforcement phases, and so on.
- ↑ D.R Katti, S.M. Pradhan, K.S. Katti, Rev. Adv. Mater Sci. 6(2004) 162.
- ↑ L.J. Gibson, M.F. Ashby, Cellular Solids: Structure and Properties – Second Edition. Cambridge University Press, Cambridge, U.K., 1997.
Citation: H. Rhee, M.F. Horstemeyer, Y. Hwang, H. Lim, H. El Kadiri, and W. Trim, “A study on the structure and mechanical behavior of the Terrapene carolina carapace: a pathway to design bio-inspired synthetic composites,” Materials Science and Engineering C 29 (2009) 2333-2339.